N A N O E X P R E S S
Structural Characterization of Mesoporous Silica Nanofibers
Synthesized Within Porous Alumina Membranes
Zhihong GongÆ Guangbin JiÆ Mingbo ZhengÆ
Xiaofeng ChangÆWeijie Dai ÆLijia PanÆ
Yi ShiÆYoudou Zheng
Received: 29 May 2009 / Accepted: 3 July 2009 / Published online: 14 July 2009
Óto the authors 2009
Abstract Mesoporous silica nanofibers were synthesized within the pores of the anodic aluminum oxide template using a simple sol–gel method. Transmission electron microscopy investigation indicated that the concentration of the structure-directing agent (EO20PO70EO20) had a significant impact on the mesostructure of mesoporous silica nanofibers. Samples with alignment of nanochannels along the axis of mesoporous silica nanofibers could be formed under the P123 concentration of 0.15 mg/mL. When the P123 concentration increased to 0.3 mg/mL, samples with a circular lamellar mesostructure could be obtained. The mechanism for the effect of the P123 concentration on the mesostructure of mesoporous silica nanofibres was proposed and discussed.
Keywords Mesoporous silicaNanofiberAnodic aluminum oxideP123Template synthesis
Mesoporous materials with ordered nanochannels, tunable pore size from 2 to 50 nm, large surface area, and high hydrothermal and thermal stability have rapidly sprang up since 1990s [1, 2]. Numerous research works about
mesoporous materials have been reported, such as SiO2 [3, 4], TiO2 [5,6], carbon [7, 8], NiO [9, 10], and ZnO [11, 12]. Among these materials, mesoporous silica is widespread due to their ultrafine nanograin, highly efficient catalysis and separation [13–15]. With the development of nanotechnology, it is expected to synthesize 1-Dimensional (1D) mesoporous silica with orderly arranged and vertical nanochannel structure because of their potential applications such as waveguides , lasers , and templates that are used to grow functionalized ultrafine nanowire arrays [18,
19]. Among the different preparation procedures, the tem-plate method was widely adopted [20,21]. Compared with other templates, porous anodic aluminum oxide (AAO) membranes have orderly arranged and vertical 1D channel structure. Previously, several research groups have synthe-sized mesoporous silica nanofibers (MSNFs) within the pores of the AAO templates [22–29].
Different mesostructures of MSNFs, such as a circular hexagonal column, a circular lamellar cylinder, and a parallel hexagonal column, have been synthesized by the different preparation procedures. It is difficult to obtain the desired mesostructures for MSNFs within the AAO tem-plates. Because several parameters, such as the size of the AAO template nanochannels, the surfactant, the hydro-philicity/hydrophobicity of the channel wall, and the pre-cursor compositions, play key roles in the formation of the pore size, the orientation, and the morphology of MSNFs. Wu et al.  synthesized MSNFs with chiral mesopores such as single and double helical geometries inside the AAO membranes. Different mesostructures of MSNFs were obtained by controlling the pore size of AAO mem-branes. Yamaguchi et al. prepared MSNFs with 1D, 3D, and the mixture of 1D and 3D alignments of the silica-nanochannels. They reported that the mesostructure of MSNFs could be tuned by experimental conditions (aging Z. GongG. Ji (&)M. ZhengX. ChangW. Dai
Nanomaterials Research Institute, College of Material Science and Technology, Nanjing University of Aeronautics and Astronautics, 210016 Nanjing, People’s Republic of China e-mail: email@example.com
G. JiL. PanY. ShiY. Zheng
time and temperature) for preparing the precursor solution . Wang et al. found that the mesostructure of MSNFs was sensitive to the AAO template structure and aging conditions . Platschek et al.  systematically inves-tigated the effect of interfacial interactions and inorganic salt addition upon the orientation of MSNFs nanochannels. MSNFs with a 2D columnar hexagonal structure, a 2D circular hexagonal structure, and a mixture of 2D columnar and circular hexagonal structure were obtained by using different surfactants. However, to the best of our knowl-edge, a systematic study of the effect of the concentration of surfactant on the mesostructure of MSNFs in the con-fined space of the AAO nanochannels is rare.
Herein, we report a simple sol–gel method to synthesize MSNFs within the AAO templates. It is found that the mesostructure of MSNFs in the confined space of the AAO nanochannel was influenced by the concentration (varied from 0.1 to 0.4 mg/mL) of the P123 surfactant.
The commercially available AAO membranes (Whatman, Anodisc 47) with a nominal pore diameter of 250 nm and 60lm thickness were used as templates. The surfactant poly (ethylene oxide)-b-poly (propylene oxide)-b-poly (ethylene oxide) block copolymer EO20PO70EO20(Pluronic P123) was purchased from Sigma–Aldrich. The precursor solution was prepared according to the literature  with some modifications. Firstly, a mixture of P123 (0.4–1.6 g) and ethanol solution (40 mL) was stirred at room temper-ature until the P123 surfactant has dissolved completely in ethanol. Secondly, tetraethyl orthosilicate (TEOS: 0.93 g) was added to the mixture solution. The resultant mixture solution was continued to stir at room temperature for 10 min. The precursor solution was obtained after adding 0.4 g of hydrochloric acid (38%) to the P123/TEOS mixture solution and stirring at room temperature for 10 min. Then, the AAO template was added into the precursor solution at room temperature. After the ethanol vaporized completely, the AAO membrane was taken out from the sol, and the residual sol on the surface was completely scratched away. Then, the AAO template including the precursor was dried at 60°C for 12 h in air. A calcination process was carried out at 400°C in air for 3 h with a heating rate of 1°C/min. The as-prepared MSNFs using 0.1, 0.15, 0.2, 0.225, 0.3, 0.35, and 0.4 mg/mL of P123 in the precursor solu-tion were denoted as MSNFs-1, MSNFs-2, MSNFs-3, MSNFs-4, MSNFs-5, MSNFs-6, and MSNFs-7, respec-tively. The AAO template including MSNFs was denoted as AAO/MSNFs.
The morphology of MSNFs was observed by field emission scanning electron microscope (FE-SEM, JEOL S4800 and Gemini LEO 1530) with attached energy dispersive spec-trometry (EDS) and transmission electron microscope (TEM, JEOL JEM 2100). For the SEM measurement, a small piece of AAO/MSNFs was slightly etched by immersing into an aqueous solution of 7 wt% H3PO4 for 12 h to obtain a clear top view. Meanwhile, in order to observe the MSNFs formed inside the pore of AAO membrane, the AAO/MSNFSs was immersed into an aqueous solution of 7 wt% H3PO4 for 4 days at room temperature for removing the AAO membrane completely. Then, the samples were washed with distilled water for several times. For the TEM investigation, the AAO/MSNFs were immersed into an aqueous solution of 7 wt% H3PO4 for 4 days at room temperature and dispersed in absolute ethanol; then, a small drop of solution was placed on Cu grids covered with carbon film. N2adsorption–desorption analysis was measured on a Micrometrics ASAP2010 instrument.
Results and Discussion
The Morphology Characterization of the MSNFs
SEM observation was used to characterize the morphology feature of the as-prepared MSNFs. The top-view SEM image (see Fig.1a) of the sample clearly shows that most of the pores of AAO membranes are filled with MSNFs. Also, we observed the spaces between MSNFs and the walls of the pores of AAO membrane due to the contrac-tion under the drying and calcinacontrac-tion processes, which corresponds to the previous report . Figure1b, c, and d shows the bundle-shaped MSNFs after removal of the AAO membrane. The average diameter of each MSNFs is about 200 nm, which mainly depends on the pore size of the AAO membrane.
the sample with a circular lamellar mesostructure sym-metrically along the edges and a circular columnar meso-structure in the central region is observed in Fig.2e. This mesostructure attributes to the confined growth of the cir-cular columnar mesostructure inside the pores of the AAO membrane, and it is made up of a circular multilayered lamellar mesostructure filled around the AAO nanochan-nel. When the concentration of P123 increase to 0.3 or 0.35 mg/mL, only a circular lamellar mesostructure can be found due to the formation of the circular columnar mes-ostructure is suppressed (Fig.2f, g, and h). Obviously, the silica circular layers are coaxially oriented within MSNFs. The layer-to-layer distance is estimated around 30–50 nm. Figure2e and g indicate that the mesostructure of MSNFSs-4 is a transitional structure from a circular colum-nar mesostructure to a circular lamellar mesostructure. The TEM results clearly indicate that the mesostructure of MSNFs can significantly be affected by the concentration of P123 in the precursor solution. The schematic illustra-tion in Fig.3 describes the inner structural transformation of MSNFs with the varying the concentrations of P123 (0.15, 0.225, and 0.3 mg/mL). Although the complicated mesostructures of MSNFs in Fig.2a, d, and i were not described in the schematic illustration because of their complicated structures, these complicated mesostructures indicated that the mesostructure of MSNFs was changed by varying the concentration of P123. Under the confined space of the AAO nanochannels, three representative
mesostructures for MSNFs were obtained by varying the concentration of P123. When the concentration of P123 was 0.15 mg/mL, MSNFs-2 was composed of columned nanochannels (Fig.3a). The orientation of nanochannels paralleled the long axis of the AAO nanochannel. With the concentration of P123 increasing to 0.225 mg/mL, two types of mesostructures formed in MSNFs-4 (Fig. 3b). These were the columned mesopores with the orientation of nanochannel circling the axis of the AAO nanochannels and the concentric multilayered lamellar mesostructure. MSNFs-5 with the concentric multilayered lamellar mes-ostructure formed, when the concentration of P123 increased to 0.3 mg/mL (Fig.3c).
It is well known that the shape of the micelles formed in the aqueous solutions dramatically depends on the concen-tration and the temperature. The relationship of the con-centration with the structure has been investigated widely by dynamic light scattering (DLS), pulsed-field-gradient NMR, and so forth [34–40]. Take the typical triblock copolymer (P123) for an example, various morphologies of the micelles, such as spherical, cylindrical, and lamellar, can be obtained by using different concentrations of the surfactant (P123), because of the hydrophobic and hydrophilic inter-action between the inner and outer region in a micelle. Wanka et al.  studied the phase diagrams and aggrega-tion behavior of poly (oxyethylene)-poly (oxypropylene)– poly (oxyethylene) triblock copolymers in aqueous solution. They found that block copolymers exhibit a rich variety of
equilibrium symmetries (spherical, cylindrical, and lamel-lar) that could be controlled by varying the concentration and the temperature.
Meanwhile, the confinement effects are also important to the morphology of a micelle. Stucky et al.  reported that in a physically confined environment, interfacial interactions, symmetry breaking, structural frustration, and confinement-induced entropy loss could play dominant roles in determining molecular organization.
In this present work, several complicated mesostructures displayed in Fig.2a, d, and i have been observed. Although the mechanism was not very clear, it is considered that these results could possibly be ascribed by the effects of both the concentration of surfactant and the confined space, because of the fact that some simple mesostructures, such as the mixture of cylindrical and lamellar, the alignment of nanochannels, and the circular lamellar, have been fabri-cated by using different amount of P123 in ethanol solu-tion, and the results are in agreement with the previous reported [30,31,33]. Thus, we propose that the phase of the surfactant (P123) micelles has significant impact on the mesostructure of MSNFs in the confined space of the AAO
Fig. 3 Schematic diagrams concerning the change in the
mesostruc-ture of MSNFs with increasing the concentrations of P123: (a) 0.15 mg/mL; (b) 0.225 mg/mL; and (c) 0.3 mg/mL
0.0 0.2 0.4 0.6 0.8 1.0
20 30 40 50 60 70 80
Relative Pressure P/P0
0 10 20 30 40 50
0.0000 0.0002 0.0004 0.0006 0.0008 0.0010
Pore diameter (nm)
0.0 0.2 0.4 0.6 0.8 1.0
5 10 15 20 25 30 35
Adsorbed Volume (cm
Relative Pressure (P/P0)
0 10 20 30 40 50 60 70 80 90 100110120130140150 0.0000
0.0001 0.0002 0.0003 0.0004 0.0005 0.0006 0.0007
Pore diameter (nm)
nanochannel under the same others experimentation condition.
N2Adsorption–Desorption Isotherms Analysis
Figure4shows the N2adsorption–desorption isotherms and the pore-size distribution curves for AAO/MSNFs-2 and AAO/MSNFs-5, respectively. Figure4a and c shows the type IV with type H4 hysteresis loops, which are typical for mesoporous materials. There are dissimilarities for the two N2adsorption–desorption isotherms, which is possibly due to the different nanochannel structure of MSNFs. Figure4b and d shows the pore-size distribution curves of AAO/ MSNFs-2 and AAO/MSNFs-5, which are in agreement with the results of TEM analysis. From the distribution curves, the sample AAO/MSNFs-2 has a narrow distribution in the range of 5–10 nm (Fig.4b). For the sample AAO/MSNFs-2, a broad pore-size distribution is observed (Fig.4d). Mean-while, the pore volumes for AAO/MSNFs-2 and AAO/ MSNFs-5 are estimated to be 0.110 and 0.048 cm3/g, respectively. The Brunauer–Emmett–Teller (BET) surface area for AAO/MSNFs-2 and AAO/MSNFs-5 are estimated to be 73.0 and 28.7 m2/g, respectively.
In summary, MSNFs have been prepared within the pores of the AAO templates using a simple sol–gel method. At the same time, we found that MSNFs with alignment of the silica-nanochannels, a circular lamellar cylinder and other complicated mesostructures could be regulated by control-ling the concentration of P123 in the precursor solution. It is considered that the phase of P123 micelles has a significant impact on the mesostructure of MSNFs in the confined space of the AAO nanochannels. The extensive structural control achieved for the mesoporous silica has a potential applica-tion to a wide variety of fields such as catalysis, adsorpapplica-tion, separation, nanoelectronic, and nanooptic.
Acknowledgments Financial support from the National Natural
Science Foundation of China (50701024), National Key Project of Fundamental Research (973, No. 2007CB936300), China Postdoc-toral Science Foundation (20080430164 and 200801366), and Jiangsu Postdoctoral Science Foundation (0801040B) are gratefully acknowledged.
1. D.Y. Zhao, J.L. Feng, Q.S. Huo, B. Melose, G.H. Fredrickson, B.F. Chmelka, G.D. Stucky, Science279, 548 (1998)
2. D.Y. Zhao, Q.S. Huo, J.L. Feng, B.F. Chmelka, G.D. Stucky, J. Am. Chem. Soc.120, 6024 (1998)
3. H.R. Byon, B. Chung, T. Chang, H.C. Choi, Chem. Mater.20, 6600 (2008)
4. E. Bloch, P.L. Llewellyn, T. Phan, D. Bertin, V. Hornebecq, Chem. Mater.21, 48 (2009)
5. I. Bannat, K. Wessels, T. Oekermann, J. Rathousky, D. Bahne-mann, M. Wark, Chem. Mater.21, 1645 (2009)
6. M.C. Tsai, J.C. Chang, H.S. Sheu, H.T. Chiu, C.H. Lee, Chem. Mater.21, 499 (2009)
7. C. Song, J.P. Du, J.H. Zhao, S. Feng, G.X. Du, Z.P. Zhu, Chem. Mater.21, 1524 (2009)
8. A. Stein, Z.Y. Wang, M.A. Fierke, Adv. Mater21, 265 (2009) 9. W. Yue, W.Z. Zhou, Chem. Mater.19, 2359 (2007)
10. J.R.A. Sietsma, J.D. Meeldijk, M. Versluijs-Helder, A. Broersma, A. Jos van Dillen, P.E. de Jongh, K.P. de Jong, Chem. Mater.20, 2921 (2008)
11. D. Chandra, S. Mridha, D. Basak and A. Bhaumik, Chem. Commun., 2384 (2009)
12. Y.Y. Song, X.B. Cao, Y. Guo, P. Chen, Q.R. Zhao, G.Z. Shen, Chem. Mater.21, 68 (2009)
13. Y.J. Han, J.M. Kim, G.D. Stucky, Chem. Mater.12, 2068 (2000) 14. J. Lee, J.C. Park, H. Song, Adv. Mater.20, 1532 (2008) 15. J. W. Zhao, F. Gao, Y. L. Fu, W. Jin, P. G. Yang, D. Y. Zhao,
Chem. Commun., 752 (2002)
16. Q.S. Huo, D.Y. Zhao, J.L. Feng, K. Weston, S.K. Buratto, G.D. Stucky, S. Schacht, F. Schueth, Adv. Mater.9, 974 (1997) 17. J. Loerke, F. Marlow, Adv. Mater.14, 1745 (2002)
18. Y.Y. Wu, G.S. Cheng, K. Katsov, S.W. Sides, J.F. Wang, J. Tang, G.H. Fredrickson, M. Moskovits, G.D. Stucky, Nature Mater.3, 816 (2004)
19. Y.Y. Wu, T. Livnch, Y.X. Zhang, G.S. Cheng, J.F. Wang, J. Tang, M. Moskovits, G.D. Stucky, Nano Lett.4, 2337 (2004) 20. M. Steinhart, J.H. Wendorff, A. Greiner, R.B. Wehrspohn, K.
Nielsch, J. Schilling, J. Choi, U. Gosele, Science296, 1997 (2002) 21. C.P. Li, B.K. Teo, X.H. Sun, N.B. Wong, S.T. Lee, Chem. Mater.
17, 5780 (2005)
22. Z.L. Yang, Z.W. Niu, X.Y. Gao, Z.Z. Yang, Y.F. Lu, Z.B. Hu, C.C. Han, Angew. Chem. Int. Ed.42, 4201 (2003)
23. Q.Y. Lu, F. Gao, S. Komarneni, T.E. Mallouk, J. Am. Chem. Soc. 126, 8650 (2004)
24. G. Kickelbick, Small1, 168 (2005)
25. W.S. Chae, S.W. Lee, Y.R. Kim, Chem. Mater.17, 3072 (2005) 26. B. Platschek, N. Petkov, T. Bein, Angew. Chem. Int. Ed.45, 1134
27. S. Yoo, M.D. David, D.F. Shantz, Langmuir22, 1839 (2006) 28. N. Petkov, B. Platschek, M.A. Morris, J.D. Holmes, T. Bein,
Chem. Mater.19, 1376 (2007)
29. V. Cauda, L. Muhlstein, B. Onida, T. Bein, Micro. Meso. Mater. 118, 435 (2009)
30. A. Yamaguchi, H. Kaneda, W. Fu, N. Teramae, Adv. Mater.20, 1034 (2008)
31. K. Jin, B.D. Yao, N. Wang, Chem. Phys. Lett.409, 172 (2005) 32. B. Platschek, N. Petkov, D. Himsl, S. Zimdars, Z. Li, R. Ko¨hn, T.
Bein, J. Am. Chem. Soc.51, 17362 (2008)
33. D.H. Wang, R. Kou, Z.L. Yang, J.B. He, Z.Z. Yang, Y.F. Lu, Chem. Commun.2, 166 (2005)
34. P. Alexandridis, T. Alan Hatton, Colloids Surf. A: Physicochem. Eng. Asp.96, 1 (1995)
35. Z. Zhou, B. Chu, J. Colloid Interface Sci.126, 171 (1988) 36. P. Mukerjee, K.J. Mysels, Critical micelle concentrations of
aqueous surfactant systems, NSRDS-NBS 36 (Government Printing Office, Washington, DC, 1971)
37. A. Sikora, Z. Tuzar, Makromol. Chem.184, 2049 (1983) 38. C. Price, Pure Appl. Chem.55, 1563 (1983)
39. P. Linse, M. Malmsten, Macromolecules25, 5434 (1992) 40. N.K. Reddy, P.J. Fordham, D. Attwood, C. Booth, Chem. Soc.,
Faraday Trans.86, 1569 (1991)